Scaffolds serving as nerve conduits.
Marine polysaccharides (e.g., chitosan, alginate and agarose) meet the requirements of artificial nerve grafting. These include the following: (1) prerequisites of biopolymers used as scaffolds; (2) conditions required by nerve autografts; (3) macroengineering requirements (form, design); (4) microengineering requirements (microgrooves, inclusion filaments); (5) mechanical conditions required by nerve autografts; (6) molecular aspects of peripheral nerve regeneration; space and adherence for: (i) chondroitin sulfate proteoglycans, (ii) neurite outgrowth promoting factors, (iii) neurotrophic factors, (iv) cells; (7) artificial side grafts should be compatible with autologous nerve grafts; (8) spatial distribution of neurotrophic factor gradients; (9) modulation of fibrosis; (10) renewal of luminal fillers. The mechanical stability of chitosan should be increased by adding other polymeric chains and cross-linking. As a result of deacetylation of chitin, chitosan scaffolds have got numerous positively charged free amino groups that provide adherence for growth factors and cells. To modulate fibrosis, heparin cross-linked chitosan microspheres have proved effective for delivering/transplanting cells, heparin and growth factors. To renew luminal fillers, chitosan microspheres may be injected through an indwelling catheter incorporated into the nerve conduit. Agarose and alginate have gained more acceptance as hydrogel lumen fillers. Interacting with positively charged chitosan, negatively charged alginate may form versatile chitosan-calcium-alginate microspheres.
- nerve grafting
- side grafting
- brachial plexus lesions
- artificial nerve grafts
After brachial plexus traction injuries, the nerve gap may be too large to be bridged by autogenous nerve grafts alone. This has prompted neuroscientists to investigate the use of artificial nerve grafts. Materials used as scaffolds for these grafts are summarized in Table 1 [1–4]. Biodegradable materials have displaced nondegradable silicone nerve conduits because these have been associated with a chronic tissue response and poor regeneration [4–6]. Several tube and sheet forms are readily available on the market for use in peripheral nerve repair [e.g., Neurotube [polyglycolic acid (PGA), Synovis], Neurolac (poly-dl-lactide-caprolactone, PLCL, Polyganics BV), NeuraGen (collagen type I, Integra NeuroSciences) and Neuro-Matrix/Neuroflex (collagen type I, Collagen Matrix Inc) [7–10]. The degradation rate of these conduits typically ranges from months (Neurotube in 3 months and NeuroMatrix in 7 months to years; Neurolac in 16 months and NeuraGen in 4 years) [4, 11]. A few of these resorbable conduits have been tested clinically in short nerve defects [2, 12–15]. Comparable or even superior results have been reported compared to nerve autografts [13, 15, 16]. In reconstructing long nerve defects, Neurolac and NeuraGen nerve conduits have induced functional recovery similar to nerve autografts [4, 17, 18]. Nevertheless, use of nerve conduits has been limited to nerve gaps less than 3 cm in length [2, 19]. Because of this, their clinical use has been limited, especially in brachial plexus lesions.
2.1. Nerve allografts
2.2. Decellularized biomatrices
2.3. Conduits consisting of basal laminae
2.4. Natural polymers; in vivo extracellular matrix polymers
2.4.2. The glycosaminoglycan hyaluronic acid. Hyaluronic acid has been developed into an extremely useful copolymer gel with methylcellulose
2.5. Natural polymers; polymers derived from blood
2.5.1. Plasma derived polymers
2.6. Natural polymers; polymers from marine life
2.6.1. Agarose is a linear polysaccharide derived from seaweed and cross-linked by temperature gradients through hydrogen bonding
2.6.2. Alginate is obtained from algae and the polymer solution is cross-linked by calcium into a sponge-like structure
2.6.3. Chitosan is a glycosaminoglycan (GAG) carbohydrate polymer derived by chemical deacetylation of chitin, the major structural polysaccharide found in crustacean, shellfish and insect shells
2.6.7. Hyaluronans, chondroitin sulfates, dermatan sulfates, heparan sulfates, keratin sulfates
3.2. Polytetrafluoroethylene (ePTFE)
3.4. Longitudinally oriented suture material (silk)
4.1. Aliphatic polyesters
Members of this family include polyglycolic acid PGA, poly(lactic acid) (PLA), polycaprolactone (PCL) and their copolymers like PLGA
4.2. Poly(phosphor)esters (PPE)
Such polymers contain a characteristic phosphoester linkage in the backbone, which is more easily cleaved via hydrolysis in physiologically relevant conditions than the ester linkage. One type is poly(bis(hydroxyethyl) terephthalate-ethylphosphoester). Another one is poly(caprolactone-co-ethyl ethylene phosphate) (PCLEEP)
DegraPol is an example. It is synthesized by coupling poly(R-3-hydroxybutyric acid-co-R-3-hydroxyvaleric acid)-diol and poly(glycolide-co-caprolactone)-diol (PGCL) with 2, 2, 4-trimethylhexamethylene diisocyanate
4.4. Hydrogel-based conduits
These are based on polyethyleneglycol, a biodegradable synthetic polymer of ethylene oxide units. Hydrogel tubes are fabricated from poly(2- hydroxyethyl methacrylate) (PHEMA). PHEMA homopolymer may be copolymerized with methyl methacrylate (MMA) to provide greater rigidity. These PHEMA-MMA tubes have a biphasic wall structure, with an outer gel-like layer and inner porous layer
4.5. Piezoelectric polymers
Poled poly(vinylidene fluoride) (PVDF) conduits are fabricated by stretching PVDF conduits (to mechanically align dipoles) and then subjecting them to an electric field nA copolymer of PVDF and trifluoroethylene (PVDF–TFE) does not require mechanical stretching to align the dipoles. Positively poled PVDF–TFE conduits have shown the best results
The clinical use of artificial nerve grafts has gained new impetus, however. First, advances in conduit lumen filler technology have made it possible to use nerve scaffolds to bridge large peripheral nerve defects . Second, after conventional end-to-end grafting, side grafting has made it possible to increase the incidence of nerve regeneration by applying additional (artificial) grafts extending from the side of the donor end to the side of the recipient end, so-called co-grafting . Third, the axonal growth cone has been found to be sensitive to spatial molecular concentration gradients of nerve growth factors [22, 23]. Thus, artificial nerve side grafts supplied with spatial molecular concentration gradients of nerve growth factors might not only act as additional grafts to autografts but might provide additional stimulation to axonal growth cone progression within autografts as well. This might provide a solution for limited axonal progression in long-standing lesions (of more than one-year duration) or for partially regenerated lesions (obstetric brachial plexus lesions after 3 years of age). In light of these findings and expectations, the requirements of an artificial nerve graft have to be redefined. Marine polysaccharides (chitosan, alginate and agarose) may be modified or combined with other polymers, thus offering wide versatility to meet these requirements.
2. Requirements of an artificial nerve graft
Biopolymer scaffolds used as artificial nerve grafts should be biocompatible; their absorption and degradation kinetics should match the degree of in vivo cell/tissue growth; they should have adequate surface for cell access, proliferation and cell differentiation and lastly, they should not be toxic or carcinogenic; the same applies to their degradation products . In addition, they should meet specific requirements
2.1. Artificial nerve grafts should fulfill the same conditions required by nerve autografts
In 1943, Seddon recognized three nerve injury types as follows: neuropraxia, axonotmesis and neurotmesis . In 1951, Sunderland [25, 26] elaborated on this classification recognizing five degrees of nerve injury. A sixth degree has recently been added by Mackinnon . Millesi  has subclassified Sunderland’s classification according to the degree of fibrosis (Table 1). Autogenous nerve grafting is the standard for repair of irreducible nerve gaps (Millesi Subtypes 3C, 4N, 4S; Sunderland Type 5, Mackinnon Type 6) . Autogenous grafts act as immunogenically inert scaffolds for axonal cone progression, providing simultaneously neurotrophic factors and Schwann cells for axonal regeneration .
2.1.1. Artificial nerve grafts should meet macroengineering requirements
To act as interposition nerve grafts, biomaterial polymer nerve scaffolds should meet macroengineering requirements, that is, they should be of proper form, design (shape) and size (diameter). In addition, they should be supplied with macrogrooves and have reasonable wall thickness. As to
2.1.2. Artificial nerve grafts should meet microengineering requirements
Microengineering refers primarily to microgrooves directing axonal growth [35–37]. Microgrooves can be placed in the polymer surface by laser etching. A minimum groove depth of 2 μm , associated with narrow ridges (5 versus 10 μm) have improved neurite outgrowth and promoted cell adhesion . Further improvements in neurite outgrowth can be obtained with coating the grooved surface with collagen or laminin peptides [40–42].
Another microengineering aspect refers to axonal preference to grow along the length of micro and nanofibers of polymers . The inclusion of filaments into the lumen of large tube diameter silicone tubes has been suggested by Lundborg et al. . The aim has been to increase the overall cross-sectional area of the regenerated nerve fibers. Itoh et al.  have used eight collagen or polyester filaments. Synthetic or biological filament lumen fillers have been used ever since to enhance nerve regeneration (Figure 2a and b). Increasing the whole filament surface area by increasing their number and reducing their diameter (increased surface area-to-volume ratio) is a serious consideration [4, 43–47].
2.1.3. Artificial nerve grafts should fulfill the same mechanical conditions required by nerve autografts
A nerve conduit should possess sufficient toughness to resist compression or collapse, yet still be flexible and suturable [4, 48]. Ideally, a nerve conduit should have an elastic modulus comparable with that of a nerve autograft. In end-to-end grafting, nerve end/artificial graft elastic or shear modulus inequality might produce tension, compression or shear at the repair site, ending up with fibrosis and hampering progression of regeneration. Such inequality might also lead to rupture of the small caliber sutures (nylon or prolene 9/0 or 10/0 sutures) used for fascicular grafting. On the contrary, during side grafting, cografting with an artificial graft of slightly higher modulus of elasticity (e.g., 64.3–69.8 MPa PLLA versus 11.7 MPa peripheral nerve tensile strength [48, 49]) aids in absorbing tension off the nerve ends and off the autograft. This may improve regeneration [50, 51] (Figures 3a–c and 4a–c).
2.2. Requirements based on molecular aspects of peripheral nerve regeneration
Biomaterial polymer nerve scaffolds should provide adequate space and adherence for the following: (1)
To provide adequate space and adherence for cells and molecules, biomaterial polymer nerve scaffolds should be porous . Currently, ideal scaffolding should have 80–90% porosity with a pore size of 50–250 μm. Its pores should be interconnected so as to allow for the introduction of lumen fillers [24, 55]. Lumen filler technology allows for incorporation of cells and molecular factors into nerve conduits using intermediary supporting matrices; its methods have been reviewed elsewhere (Figure 2a and b) . One method involves incorporating
2.3. Requirements based on recent findings of side grafting (cografting autologous nerve grafts with biomaterial polymer nerve scaffolds)
In side grafting, the donor side is grafted to the recipient end; donor side collateral sprouting is stimulated by mechanical trauma or axotomy . Similarly, the incidence of nerve regeneration after conventional end-to-end grafting can be increased by applying biomaterial polymer nerve side grafts extending from the side of the donor end to the side of the recipient end  (Figure 3c). Cografting autologous nerve grafts with biomaterial polymer nerve scaffolds presupposes biocompatibility between both.
2.4. Requirements based on spatial distribution of neurotrophic factor gradients
The axonal growth cone is sensitive to spatial molecular concentration gradients . In a study by Rosoff et al. , axonal growth has been shown to be enhanced by a steep nerve growth factor (NGF) spatial concentration gradient. Axonal growth cones also preferentially advance up gradients of laminin . For the spinal cord, gradients have been made in natural and synthetic polymers with laminin [1, 60]. Utilizing biomaterial polymer nerve scaffolds, axonal growth can be hypothetically made to bridge the whole length of the neural gap by seeding the scaffolds with multiple NGF spatial concentration gradients . By diffusion, these NGF spatial concentration gradients might also enhance axonal growth within the adjacent natural nerve side and end-to-end autografts (Figure 6).
2.5. Requirements based on modulation of fibrosis
Scar formation prevents progression of axonal regeneration. Lysing the fibrosis/gliosis in the injury zone to an extent that allows settling of the basal lamina preventing meanwhile collapse of the neural tissue matrix is therefore essential. Recognizing this, Millesi  has modified Sunderland’s classification of nerve injuries based on the degree of epineurial, perineurial and endoneurial fibrosis (Table 2). Clinically, surgical neurolysis of brachial plexus lesions has proven to be an effective procedure [50, 51, 61]. Heparin has been used for a long time in plastic surgery to lyse scar tissue . Its perineural application has improved functional recovery . Among other actions, heparin influences fibroblast growth factor responsible for cell proliferation, differentiation, signal transduction and angiogenesis [64–66]. In the central nervous system, injured axons encounter a series of inhibitory factors . Chondroitinase ABC lyses chondroitin sulfate proteoglycans allowing regenerating axons to progress to distal targets [68–70].
|Seddon type||Sunderland type-millesi subtype|
|Neuropraxia||Sunderland type 1—there is transient conduction block without disruption of the anatomical structure of the nerve. Wallerian degeneration does not occur distal to the injury. Full nerve function is expected without intervention within 12 weeks|
|Millesi subtype 1A—there is fibrosis of the epifascicular epineurium, necessitating an epineurotomy to enhance regeneration|
|Millesi subtype 1B—there is fibrosis of the interfascicular epineurium, necessitating a partial epineurectomy to enhance regeneration|
|Axonotmesis: the axons|
and Wallerian degeneration occurs
|Sunderland type 2—the endoneurim and perineurium are intact and complete regeneration and functional recovery occurs.|
|Millesi subtype 2A—there is fibrosis of the epifascicular epineurium, necessitating an epineurotomy to enhance regeneration|
|Millesi subtype 2B. There is fibrosis of the interfascicular epineurium, necessitating a partial epineurectomy to enhance regeneration|
|Sunderland type 3—the axon and endoneurium are damaged, but then perineurium and epineurium are intact. This results in disorganized regeneration which can result in obstruction or diversion of axons from their correct paths|
|Millesi subtype 3A—there is fibrosis of epifascicular epineurium, necessitating an epineurotomy to enhance regeneration|
|Millesi subtype 3B—there is fibrosis of the interfascicular epineurium, necessitating a partial epineurectomy to enhance regeneration|
|Millesi subtype 3C—there is additional endoneural fibrosis. During surgery, electric stimulation of the affected nerve shows poor contraction of the muscle(s) supplied by it. Treatment is by excision of the fibrotic segment and nerve grafting|
|Sunderland type 4—fourth degree injuries involve damage to all structures, however, continuity of the nerve trunk is bridged by a mass of connective tissue, Schwann cells and regenerating axons. Conduction down the nerve is not possible|
|Millesi subtype 4N. The scar is invaded by neuroma. During surgery, electric stimulation of the affected nerve shows decreased or lost contraction of the muscle(s) supplied by it. Treatment is accordingly surgical by neurolysis or excision and nerve grafting|
|Millesi subtype 4S—the scar consists of fibrosis only. During surgery, electric stimulation of the affected nerve shows lost contraction of the muscle(s) supplied by it. Treatment is surgical by excision and nerve grafting|
|Neurotmesis (complete division of|
|Sunderland type 5—the continuity of the nerve/brachial plexus roots, trunks, divisions or cords is completely interrupted. There may be brachial plexus root avulsions. Root avulsions are excluded by myelography or intraoperative foraminotomy. During surgery, electric stimulation of the interrupted nerve shows lost contraction of the muscle(s) supplied by it. Treatment is surgical by excision and nerve grafting, or by nerve transfer in root avulsions|
|MacKinnon type 6—a sixth degree of injury has been described by MacKinnon . This refers to lesions with a mixed pattern of injury where there are varying degrees of injury in different sections of the nerve|
Can we use artificial nerve side grafts supplied with spatial molecular concentration gradients of nerve growth factors for the following purposes simultaneously:
- to act as additional side grafts to end-to-end autografts as discussed under ‘ requirements based on recent findings of side grafting’,
- to stimulate axonal growth cone progression within end-to-end autografts as discussed under ‘requirements based on spatial distribution of neurotrophic factor gradients’,
- to lyse postoperative fibrosis after brachial plexus surgery and direct cord implantation (using heparin and chondroitinase ABC respectively),
- as a result of the above, to regain full hand, elbow and shoulder functions in recent (less than 1 year) total brachial plexus palsy,
- as a result of the above, to provide a solution for limited axonal progression in long-standing brachial plexus lesions (of more than one-year duration) or for partially regenerated lesions (obstetric brachial plexus lesions after 3 years of age). This is an important consideration in view of the mounting evidence that motor endplates do not atrophy but are in a continuous regenerative process [71, 72].
Advances in lumen filling technology points to the possibility of all of the above (Figures 2a, b and 7). Use can be made of both heparin as a neurolyzing agent as well as its ligand–receptor binding property. Heparin-incorporated fibrin–fibronectin matrices can enhance nerve regeneration by binding to FGF, GDNF and NGF [73–76], preventing their enzymatic cleavage, allowing them to bind to their respective growth factor receptors with greater affinity thus improving signal transduction [77, 78] and allowing for their release at a slower rate compared to when bound to a fibrin matrix alone [79, 80].
2.6. Requirements based on the necessity of renewal (recycling) of luminal fillers to allow for the replenishment of cells, molecular factors and concentration gradients
Closely linked to the above questions, is the following question. In global brachial plexus avulsions associated with extensive fibrosis and in which the whole brachial plexus has retracted to the axilla, can we use artificial side grafts to improve the results of direct cord implantation? In such a situation, the nerve gap is extensive and associated with excessive scarring. The axonal growth cone would thus take years to reach the target muscles. Consequently, the factors mentioned before have to be replenished continually.
This can take place through a continous cell and drug delivery system (catheter) [81, 82]. Versatility is required to achieve the following three aims simultaneously: keeping the cell and drug delivery system (catheter) patent; dissolving the fibrous tissue that blocks pores after release of molecules and cells and replenishment of released molecules and cells associated with preservation of their spatial concentration gradients. Microsphere, nanosphere and nanoshell technology is one method to achieve the previous aims [1, 83, 84]. Controlling surface tension as well as hydrophobic and hydrophilic properties of the conduit lumen and the microspheres may help us fulfill the simultaneous three aims described previously (Figure 8).
3. Chitosan as a biomaterial polymer nerve scaffold
3.1. Chitosan as a biopolymer; special properties
Chitosan [poly-(β-1/4)-2-amino-2-deoxy-d-glucopyranose] [1, 24] is a
3.2. Chitosan as an artificial nerve graft scaffold fulfills the same conditions required by nerve autografts
3.2.1. Chitosan as an artificial nerve graft scaffold meets macroengineering requirements
Chitosan can be easily processed and manufactured in a variety of forms including tubes, fibers, films, sponges and hydrogels. Although nonwoven chitosan mesh conduits  and cell-seeded chitosan films  have supported axonal growth, tubes are the most common in practice, either as hollow structures or combined with lumen fillers [2, 24]. Stenberg et al.  have used hollow chitosan tubes for reconstruction of rat sciatic nerve defects. Gonzalez-Perez et al.  and others  have proven the regenerative capability of chitosan tubes of low (∼2%) and medium (∼5%) degree of acetylation, to bridge critical nerve gaps (15 mm long) in the rat sciatic nerve. Meyer et al.  have used fine-tuned chitosan nerve tubes with a longitudinal chitosan film as a lumen filler to reconstruct long sciatic nerve defects in rats. Nerve scaffolds composed of a chitosan nerve guidance conduit filled with polyglycolic acid (PGA)/polylactic-co-glycolic acid (PLGA) filaments have been used to bridge large peripheral nerve defects both experimentally and clinically .
3.2.2. Chitosan as an artificial nerve graft scaffold meets microengineering requirements
Microgrooves, microfilaments as lumen fillers and surface treatment of chitosan are microengineering procedures.
As far as
Microengineering applies also to
3.2.3. Chitosan as an artificial nerve graft scaffold fulfills the same mechanical conditions required by nerve autografts
Chitosan is brittle, fracturing easily under low energy . Several methods have been developed to improve its mechanical properties.
In the first and most reliable one, other polymeric chains are added (e.g., polyethyleneglycol, dialdehydes). Cross-linking agents possessing at least two functional reactive groups (e.g., formaldehyde, epoxides) are used to bridge all polymeric chains together (e.g., to form glutaraldehyde and glyoxal respectively) . A bio-artificial polycaprolactone (PCL)/chitosan nanofibrous scaffold has been designed and evaluated . Mechanical testing has shown that Young’s modulus and strain at break of the electrospun PCL/chitosan nanofibers are better than those of the chitosan nanofibers. Huang et al.  have used electrospun collagen-chitosan-TPU nanofibrous scaffolds The scaffolds have been cross-linked by glutaraldehyde (GTA) vapor. Wang et al.  have used formaldehyde-cross-linked chitosan conduits containing PGA filaments .
The second method makes use of the high number of positively charged amine groups consequent upon deacetylation. They are made to react with the negatively charged factors of the molecular aspects of peripheral nerve regeneration. The resulting compounds improve both the mechanical and neurotrophic aspects of chitosan. Junka et al.  have used nanofibrous scaffolds electrospun from blends of poly(caprolactone) (PCL) and chitosan. Taking advantage of the amine groups on chitosan, the surface of the scaffolds have been functionalized with laminin by carbodiimide based cross-linking. Wang et al.  have compared chitosan nano/microfibrous tubes with a deacetylation rates of 78 and 93% to each other. Chitosan nano/microfiber mesh tubes with a deacetylation rate of 93% have had sufficient mechanical properties to preserve tube space and to provide a better scaffold for cell migration and attachment. Haastert-Talini et al.  have compared chitosan tubes of varying degrees of acetylation (low—2%, medium—5%, high—20%) for bridging peripheral nerve defects. Chitosan tubes with 5% acetylation have been found to be most supportive for peripheral nerve regeneration.
The third method consists of coating chitosan tubes with a film composed of a material of high mechanical toughness. Duda et al.  have reported on composite nerve grafts with an inner 3D multichannel porous chitosan core and an outer electrospun polycaprolactone shell. Also, cellulosic fibers in nano scale have been found to be an attractive reinforcement to chitosan, producing environmental friendly composite films with improved physical properties .
In the fourth method, the scaffold shape is additionally varied. Itoh et al. [106, 107] have developed nerve scaffolds using tendon chitosan tubes or hydroxyapatite-coated tendon chitosan tubes having either a circular or triangular cross-section, as well as triangular tubes combined with laminin. The mechanical strength of triangular tubes has been found to be higher than circular tubes and the inner volume of a triangular tube tends to be larger than in circular tubes. Nerve tissue regeneration along the tube wall has been present in both the laminin and laminin peptide groups.
In the fifth method, lumen fillers have been used. Xue et al.  have used a neural scaffold that consisted of a chitosan conduit inserted with poly(lactic-co-glycolic acid) (PLGA) fibers and mesenchymal stem cells to bridge an extra-large gap in dog sciatic nerve.
3.3. Chitosan as an artificial nerve graft scaffold fulfills requirements based on molecular aspects of peripheral nerve regeneration; chitosan fulfills requirements based on spatial distribution of neurotrophic factor gradients
The interaction of chitosan and molecular aspects of peripheral nerve regeneration obeys principles of luminal filling. The principles of lumen filling can also be applied to create spatial concentration gradients of molecular factors. Three main factors determine this: the degree of deacetylation of chitosan, its porosity and chitosan biodegradation products (chitooligosaccharides).
The biodegradation products of chitosan are water-dissolvable chitooligosaccharides (COSs), which have been shown to support peripheral nerve regeneration. Jiang et al.  have demonstrated that the beneficial effect of
3.4. Chitosan as an artificial nerve graft scaffold fulfills requirements based on recent findings of side grafting
Cografting autologous nerve grafts with biomaterial polymer nerve scaffolds presupposes biocompatibility between both. Evidence for neural cell/chitosan biocompatibility comes from an animal model of multiple sclerosis developed by Hoveizi et al. . These authors have noted the role of polylactic acid/chitosan (PLA/CS) scaffold in increasing neural cell differentiation. The biocompatibility of functional Schwann cells induced from bone mesenchymal cells with a chitosan conduit membrane has been proven by Zhang et al. .
3.5. Chitosan as an artificial nerve graft scaffold fulfills requirements based on modulation of fibrosis
Firstly, through its cationic interactions, chitosan prevents secondary infection by many types of fungi, yeasts and bacteria . Secondly, chitosan exerts an antifibrotic effect by binding to collagen via hydrogen bonding and polyanionic–polycationic interactions. Thus it prevents postoperative abdominal adhesions either singly, or as a polypropylene/chitosan mesh, or even as a chitosan-gelatin modified film. Experimentally, it has been used to prevent excessive fibrosis after intestinal resection anastomosis. The feasibility of using silk fibroin and chitosan blend scaffolds for preventing excessive fibrosis after ventral hernia repair has been investigated in guinea pigs .
Thirdly, heparin, both an anticoagulant and fibrotic drug, can be incorporated into chitosan microspheres or can be used as a luminal filling matrix molecule in chitosan conduits. Heparin cross-linked chitosan microspheres for the delivery of neural stem cells and growth factors for central nervous system repair have been used by Skop et al. . This has proved effective for transplanting large numbers of neural stem cells, heparin and FGF-2. Using chitosan nerve conduits, Han et al.  have developed a basic fibroblast growth factor delivery system fabricated with heparin-incorporated fibrin-fibronectin matrices for repairing rat sciatic nerve disruptions.
3.6. Requirements based on the necessity of renewal (recycling) of luminal fillers to allow for the replenishment of cells, molecular factors and concentration gradients
Chitosan offers the versatility required in microsphere, nanosphere and nanoshell technology [1, 91] as one method to achieve three aims simultaneously: dissolving the fibrous tissue that blocks pores after release of molecules and cells as aforementioned, replenishment of released molecules and cells associated with preservation of their spatial concentration gradients and keeping the cell and drug delivery system (catheter) patent.
To replenish released molecules and cells, Zeng et al.  have incorporated chitosan microspheres into collagen-chitosan scaffolds for the controlled release of nerve growth factor. Wei et al.  have evaluated the potential of a chitosan/silk fibroin scaffold serving as a delivery vehicle for adipose-derived stem cells in neural tissue. Wang et al.  have used Schwann cells on oriented chitosan nanofiber mesh tubes as delivery vehicles. Maysinger et al.  have prepared microspheres containing ciliary neurotrophic factor (CNTF) or genetically engineered cells able to synthesize and release this cytokine. Raisi et al.  have resorted to mesenchymal stem cell-derived microvesicles to enhance sciatic nerve regeneration in the rat.
Keeping the cell and drug delivery system (catheter) patent may necessitate external coating of the nerve conduit . Part of the external coating may be made of a hydrophobic material, preventing microsphere adherence to it and thus keeping it patent. Electrically and magnetically responsive microspheres may be exposed to repulsive fields in hydrophobic areas. Indeed these microspheres have been used to enhance nerve regeneration. Qi et al.  have electrically stimulated olfactory ensheathing cells (OECs) using a biodegradable conductive composite made of conductive polypyrrole (PPy, 2.5%) and biodegradable chitosan (97.5%). Similarly, Liu et al.  have activated Schwann cells in vitro using magnetically responsive magnetic nanoparticles (MNPs) and a biodegradable chitosan-glycerophosphate polymer.
4. Other biomaterial polymer nerve scaffolds
Although agarose and alginate have also served as nerve conduit scaffolds, they have gained more acceptance as hydrogel lumen fillers. Alginate, in particular has been used both as a lumen filler and for encapsulation of cells and drugs.
4.1.1. Agarose as a biopolymer; general properties
Agarose consists of alternating units of b-D-galactopyranose and 3, 6-anhydro-a- L-galactopyranose; extracted from different sources it can have different chemical compositions depending on Sulphated L-hydroxyl group concentrations [1, 132]. Agarose is thermoresponsive, but poorly degradable
4.1.2. Agarose as a nerve scaffold
184.108.40.206. Macroengineering and microengineering requirements
Stokols and colleagues have developed agarose-based scaffolds with linear pores by using a freeze-drying process  as well as by templating . These authors have used a freeze drying method to form agarose scaffolds containing linear guidance pores with a mean diameter of 120 μm [133, 135]. This process involves the formation of ice crystals whose size and direction of growth can be controlled by the temperature gradient . Pore size in the scaffold can also be controlled by the freezing rate and pH; the faster rate the smaller the size . Integrating BDNF into the scaffold material or using BDNF-secreting mesenchymal stem cells scaffold channels, has significantly improved the scaffold’s capacity to promote regeneration . Koffler et al.  have implanted linear-channeled agarose scaffolds in spinal cord injuries, providing growing axons with linear growth paths at the lesion site and minimizing regeneration distance. The linear channels have helped regenerating axons maintain the correct mediolateral and dorsoventral position in the spinal cord.
220.127.116.11. Pore size and mechanical properties
The average pore size of agarose hydrogels is influenced by the concentration of the polymer in solution and the settling temperature. An increase in concentration results in tightly packed helices that translate to a decrease in pore size. Decreasing the settling temperature results in small pore gels with higher elastic moduli .
18.104.22.168. Molecular aspects of peripheral nerve regeneration
The interaction of agarose and molecular aspects of peripheral nerve regeneration obeys principles of luminal filling. Agarose does not provide adhesion motifs to cells and does not allow interaction between adherent cells and the entrapping matrix. However, it can be supplemented with adhesion molecules of the extracellular matrix [56, 139, 140].
In repairing injuries in the CNS, agarose-based biomaterials have also had incredible success, at least in experimental settings [133, 134]. BDNF within lipid microtubules has been incorporated into agarose scaffolds, enhancing axonal growth for the length of the scaffold but not into the distal cord . Living neurons and axonal tracts have been internalized within agarose hydrogel tubes by Cullen et al. . In a study by Gros et al. , templated agarose scaffolds have substantially enhanced the organization and distance over which long-tract axons extend through a spinal cord lesion site in the presence of combinatorial therapies, but host-scaffold reactive interfaces have limited axon re-penetration of the host.
4.1.3. Agarose as a scaffold lumen filler
In order to promote sciatic nerve regeneration across a challenging 20 mm nerve gap in rats, Dodla and Bellamkonda  have used anisotropic scaffold lumen fillers of agarose hydrogels containing gradients of laminin-1 (LN-1) and nerve growth factor (NGF) molecules. Injectable agarose hydrogels have also been implemented [70, 143]. Using multi-photon chemistry, Wylie et al.  have created 3D agarose hydrogels that incorporate two bioactive molecules (a transcription factor and a growth factor).
4.2.1. Alginate as a biopolymer; general properties
Composed of (1–4)-linked α-l-guluronate (G) and β-d-mannuronate (M) monomers, alginat
4.1.2. Alginate as a nerve scaffold
22.214.171.124. Macroengineering and microengineering requirements
Anionic in nature, alginate can be assembled with polycations into polyelectrolyte free-standing films (i.e., films with a few micrometers in thickness) which are suitable drug reservoirs of biomolecules, such as growth factors and antibiotics . Lu et al.  have reported on the use of chitin-alginate 3D microfibrous scaffolds to support efficient neuronal differentiation and maturation under chemically defined culture conditions. Ethylene diamine has been covalently cross-linked to further freeze-dried alginate, resulting in a porous foam. This has been subsequently implanted into a 7-mm sciatic nerve gap in the rat without suturing . Alginate foams have also been tested alone or in combination with a protective PGA mesh in the treatment of a 50-mm sciatic nerve defect in the cat . Alginate foams can promote nerve regeneration even without suturing to the nerve stumps, or enclosing within a tube structure .
126.96.36.199. Molecular aspects of peripheral nerve regeneration
Wnt proteins are bifunctional axon guidance molecules, several of which appear to mediate guidance of corticospinal tract axons along the spinal cord. Park et al.  have studied the effect on spinal cord regeneration by Wnt-containing alginate scaffolds. In another study [56, 150], nerve growth factor (NGF) has been cross-linked to the wall of an alginate/chitosan scaffold.
188.8.131.52. Modulation of fibrosis
Heparin can be used both as a neurolyzing agent and as a matrix lumen filling ligand-binder. A heparin/alginate gel combined with basic fibroblast growth factor but without a tubular structure  has been used as an artificial nerve graft for digital nerve repair. A matrix consisting of heparin and alginate covalently cross-linked with ethylenediamine has been produced to stabilize and control the release of growth factors .
4.2.3. Alginate as a scaffold lumen filler
184.108.40.206. Hydrogel matrix as lumen filler
Alginate hydrogels have been used as lumen fillers in association with
220.127.116.11. Encapsulated particles as lumen fillers
Cells and growth factors may be encapsulated in protective alginate microcapsules, coated with multilayers of chitosan and alginate. Poly(lactic acid) microparticles may be co-encapsulated to provide anchorage points thus promoting cell survival . Alginate encapsulation has involved, among other things, the encapsulation of olfactory ensheathing cells (OECs) , fibroblasts engineered to produce brain-derived neurotrophic factor (Fb/BDNF)  and NGF-expressing cells .
We have outlined the requirements of artificial nerve end-to-end or preferably side grafting. These include: general prerequisites of biopolymers used as scaffolds; conditions required by nerve autografting; macroengineering requirements; microengineering requirements; mechanical conditions required by nerve autografting; requirements based on molecular aspects of peripheral nerve regeneration; requirements of side grafting; requirements based on spatial distribution of neurotrophic factor gradients; requirements based on modulation of fibrosis; requirements based on the necessity of renewal of luminal fillers to allow the replenishment of cells, molecular factors and concentration gradients. We have also outlined that using nerve conduit as side grafts necessitates their design as open cylinders, so they can be easily placed around suture lines and nerve graft and so that to allow diffusion of nutrients to the autografts. Side-grafting unloads stresses from autografts and nerve ends. They allow of spreading nerve growth factor concentration gradients and dissolution of fibrosis. Chitosan satisfies all these requirements. Combined with other materials, it makes them less stiff, thus mechanically suitable as grafts. Produced as a result of deacetylation of chitin, chitosan nerve conduit scaffolds have got numerous positively charged free amino groups, which enable them to provide adherence for nerve growth factors and cells by lumen filling methods. To modulate fibrosis, heparin cross-linked chitosan microspheres have proved effective for delivering/transplanting large numbers of neural stem cells, heparin (matrix molecule and neurolyzing agent) and FGF-2. To replenish cells and growth factors, chitosan microspheres may be injected through an indwelling catheter incorporated into an external coat of the nerve conduit. The internal surface of the catheter should be hydrophobic to inhibit adherence of cells and molecules to it, preventing its blockage. Polystyrene can be used to create superhydrophobic surfaces. The real challenge remains the catheter-conduit interface. This cannot be kept hydrophobic; nevertheless, it should be kept patent. Agarose and alginate have mainly served as hydrogel lumen fillers. Alginate, in particular, has been used both as a lumen filler and for encapsulation of cells and drug. Interacting with positively charged chitosan, negatively charged alginate may form versatile chitosan-calcium-alginate microspheres. Both cationic chitosan- and anionic alginate-coated poly(dl-lactide-co-glycolide) nanoparticles  and chitosan/alginate beads  have been produced and may be useful tools for delivering cells and molecules through the catheter-conduit interface without blocking it.
Madigan NN, McMahon S, O’Brien T, Yaszemski MJ, Windebank AJ. Current tissue engineering and novel therapeutic approaches to axonal regeneration following spinal cord injury using polymer scaffolds. Respir Physiol Neurobiol. 2009 Nov 30;169(2):183–199.
Konofaos P, Ver Halen JP. Nerve repair by means of tubulization: past, present, future. J Reconstr Microsurg. 2013 Mar;29(3):149–164. doi:10.1055/s-0032-1333316. Epub 2013 Jan 9. Review. PubMed PMID: 23303520.
Lundborg G. Alternatives to autologous nerve grafts. Handchir Mikrochir Plast Chir. 2004;36:1–7.
Jiang X, Lim SH, Mao HQ, Chew SY. Current applications and future perspectives of artificial nerve conduits. Exp Neurol. 2010 May;223(1):86–101. doi:10.1016/j.expneurol.2009.09.009. Epub 2009 Sep 19. Review. PubMed PMID: 19769967.
Panseri S, Cunha C, Lowery J, Del Carro U, Taraballi F, Amadio S, Vescovi A, Gelain F. Electrospun micro- and nanofiber tubes for functional nervous regeneration in sciatic nerve transections. BMC Biotechnol. 2008;8:39.
Rangappa N, Romero A, Nelson KD, Eberhart RC, Smith GM. Laminincoated poly(L-lactide) filaments induce robust neurite growth while providing directional orientation. J Biomed Mater Res. 2000;51:625–634.
Meek MF, Coert JH. US Food and Drug Administration/Conformit Europe approved absorbable nerve conduits for clinical repair of peripheral and cranial nerves. Ann Plast Surg. 2008;60(4):466–472.
Mackinnon SE, Hudson AR, Bojanowski V, Hunter DA, Maraghi E. Peripheral nerve injection injury with purified bovine collagen—an experimental model in the rat. Ann Plast Surg. 1985;14:428–436.
Meek MF, Dunnen WFD. Porosity of the wall of a neurolac nerve conduit hampers nerve regeneration. Microsurgery. 2009;29:473–478.
Zeng W, Rong M, Hu X, Xiao W, Qi F, Huang J, Luo Z. Incorporation of chitosan microspheres into collagen-chitosan scaffolds for the controlled release of nerve growth factor. PLoS One. 2014 Jul 1;9(7):e101300. doi:10.1371/journal.pone.0101300. eCollection 2014. PubMed PMID: 24983464; PubMed Central PMCID: PMC4077743.
Schlosshauer B, Dreesmann L, Schaller HE, Sinis N. Synthetic nerve guide implants in humans: a comprehensive survey. Neurosurgery. 2006;59:740–748.
Mackinnon SE, Dellon AL. Clinical nerve reconstruction with a bioabsorbable polyglycolic acid tube. Plast Reconstr Surg. 1990;85:419–424.
Weber RA, Breidenbach WC, Brown RE, Jabaley ME, Mass DP. A randomized prospective study of polyglycolic acid conduits for digital nerve reconstruction in humans. Plast Reconstr Surg. 2000;106:1036–1045, discussion 1046–1048.
Kim J, Dellon AL. Reconstruction of a painful post-traumatic medial plantar neuroma with a bioabsorbable nerve conduit: a case report. J Foot Ankle Surg. 2001;40:318–323.
Inada Y, Morimoto S, Takakura Y, Nakamura T. Regeneration of peripheral nerve gaps with a polyglycolic acid-collagen tube. Neurosurgery. 2004;55:640–646, discussion 646–648.
Navissano M, Malan F, et al. Neurotube for facial nerve repair. Microsurgery. 2005;25(4):268–271.
Bertleff, M.J.O.E., Meek, M.F., et al.. A prospective clinical evaluation of biodegradable Neurolac nerve guides for sensory nerve repair in the hand. J Hand Surg. 2005;30(3):513–518.
Lohmeyer J, Zimmermann S, Sommer B, Machens HG, Lange T, Mailander P. Bridging peripheral nerve defects by means of nerve conduits. Chirurg. 2007;78:142–147.
Pabari A, Yang SY, Seifalian AM, Mosahebi A. Modern surgical management of peripheral nerve gap. J Plast Reconstr Aesthet Surg. 2010;63:1941–1948.
Gu X. Progress and perspectives of neural tissue engineering. Front Med. 2015;9(4):401–411. doi:10.1007/s11684-015-0415-x.
Amr SM, Moharram AN. Repair of brachial plexus lesions by end-to-side side-to-side grafting neurorrhaphy: experience based on 11 cases. Microsurgery. 2005;25(2):126–146.
Rosoff WJ, Urbach JS, Esrick MA, McAllister RG, Richards LJ, Goodhill GJ. A new chemotaxis assay shows the extreme sensitivity of axons to molecular gradients. Nat Neurosci. 2004 Jun;7(6):678–82. Epub 2004 May 25 (Erratum in: Nat Neurosci. 2004 Jul;7(7):785).
Tse TH, Chan BP, Chan CM, Lam J. Mathematical modeling of guided neurite extension in an engineered conduit with multiple concentration gradients of nerve growth factor (NGF). Ann Biomed Eng. 2007 Sep;35(9):1561–1572. Epub 2007 May 23.
Rodríguez-Vázquez M, Vega-Ruiz B, Ramos-Zúñiga R, Saldaña-Koppel DA, Quiñones-Olvera LF. Chitosan and its potential use as a scaffold for tissue engineering in regenerative medicine. Biomed Res Int. 2015;2015:8212–8279.
Chimutengwende-Gordon M, Khan W. Recent advances and developments in neural repair and regeneration for hand surgery. Open Orthopaedics J. 2012;6 (Suppl 1: M13):103–107.
Millesi H. Chirurgie der Peripheren Nerven. Munich: Urban &Schwarzenberg; 1992; pp. 14–15.
Hiroshi N, Tator CH, Shoichet MS. Bioengineered strategies for spinal cord repair. J Neurotrauma. 2006;23:496–507 [PubMed: 16629632].
Wong DY, Leveque JC, Brumblay H, Krebsbach PH, Hollister SJ, Lamarca F. Macro-architectures in spinal cord scaffold implants influence regeneration. J Neurotrauma. 2008;25:1027–1037 [PubMed: 18721107].
Krych AJ, Rooney GE, Chen B, Schermerhorn TC, Ameenuddin S, Gross L, Moore MJ, Currier BL, Spinner RJ, Friedman JA, Yaszemski MJ, Windebank AJ. Relationship between scaffold channel diameter and number of regenerating axons in the transected rat spinal cord. Acta Biomater. 2009 Sep;5(7):2551–9. doi:10.1016/j.actbio.2009.03.021. PubMed PMID: 19409869; PubMed Central PMCID:PMC2731813.
Moore MJ, Friedman JA, Lewellyn EB, Mantila SM, Krych AJ, Ameenuddin S, Knight AM, Lu L, Currier BL, Spinner RJ, Marsh RW, Windebank AJ, Yaszemski MJ. Multiple-channel scaffolds to promote spinal cord axon regeneration. Biomaterials. 2006b;27:419–429 [PubMed: 16137759].
Ducker TB, Hayes GJ. Experimental improvements in the use of Silastic cuff for peripheral nerve repair. J Neurosurg. 1968;28:582.
Rutkowski GE, Heath CA. Development of a bioartificial nerve graft. II. Nerve regeneration in vitro. Biotechnol Prog. 2002;18:373.
Kokai LE, Lin YC, Oyster NM, Marra KG. Diffusion of soluble factors through degradable polymer nerve guides: controlling manufacturing parameters. Acta Biomater. 2009;5:2540.
Nectow AR, Marra KG, Kaplan DL. Biomaterials for the development of peripheral nerve guidance conduits. Tissue Eng Part B Rev. 2012 Feb;18(1):40–50. doi:10.1089/ten.TEB.2011.0240. Epub 2011 Sep 23. Review. PubMed PMID: 21812591; PubMed Central PMCID: PMC3262974.
Bellamkonda R. Peripheral nerve regeneration: an opinion on channels, scaffolds and anisotropy. Biomaterials. 2006;27:3515–3518 [PubMed: 16533522].
Bellamkonda R, Ranieri JP, Bouche N, Aebischer P. Hydrogel-based three-dimensional matrix for neural cells. J Biomed Mater Res. 1995;29:663–671 [PubMed: 7622552].
Khademhosseini A, Langer R. Microengineered hydrogels for tissue engineering. Biomaterials. 2007;28:5087–5092 [PubMed: 17707502].
Clark P, Connolly P, Curtis A, Dow J, Wilkinson C. Cell guidance by ultafine topography in vitro. J Cell Sci. 1991;99:73–77 [PubMed: 1757503].
Goldner JS, Bruder JM, Li G, Gazzola D. Neurite bridging across micropatterned grooves. Biomaterials. 2006;27:460–472 [PubMed: 16115675].
Yao L, Damodaran G, Nikolskaya N, Gorman AM, Windebank AJ, Pandit A. The effect of laminin peptide gradient of enzymatically cross-linked collagen scaffold on neurite growth. J Biomed Mater Res A. 2009a;11 (Epub February 11, 2009).
Yao L, O’Brien N, Windebank A, Pandit A. Orienting neurite growth in electrospun fibrous neural conduits. J Biomed Mater Res B Appl Biomater. 2009b;90(2):483–491 [PubMed: 19130615].
Yao L, Wang S, Cui W, Sherlock R, O’Connell C, Damodaran G, Gorman A, Windebank A, Pandit A. Effect of functionalized micropatterned PLGA on guided neurite growth. Acta Biomater. 2009c;5:580–588 [PubMed: 18835227].
Lundborg G, Dahlin L, Dohi D, Kanje M, Terada N. A new type of “bioartificial” nerve graft for bridging extended defects in nerves. J Hand Surg (Br.). 1997;22:299–303.
Itoh S, Takakuda K, Ichinose S, Kikuchi M, Schinomiya K. A study of induction of nerve regeneration using bioabsorbable tubes. J Reconstr Microsurg. 2001;17:115–123.
Chew SY, Mi R, Hoke A, Leong KW. Aligned protein–polymer composite fibers enhance nerve regeneration: a potential tissue-engineering platform. Adv Funct Mater. 2007;17:1288–1296.
Zhang BG, Quigley AF, Myers DE, Wallace GG, Kapsa RM, Choong PF. Recent advances in nerve tissue engineering. Int J Artif Organs. 2014 Apr;37(4):277–91. doi:10.5301/ijao.5000317. Epub 2014 Apr 15. Review. PubMed PMID: 24811182.
Hudson TW, Evans GR, Schmidt CE. Engineering strategies for peripheral nerve repair. Clin Plast Surg. 1999;26:617–628, ix.
Weir NA, Buchanan FJ, Orr JF, Farrar DF, Boyd A. Processing, annealing and sterilisation of poly-L-lactide. Biomaterials. 2004;25:3939.
Rydevik BL, Kwan MK, Myers RR, Brown RA, Triggs KJ, Woo SL, Garfin SR. An in vitro mechanical and histological study of acute stretching on rabbit tibial nerve. J Orthop Res. 1990;8:694.
Millesi H. Factors affecting the outcome of peripheral nerve surgery. Microsurgery. 2006;26:295–302.
Millesi H, Rath Th, Reihsner R, Zoch G. Microsurgical neurolysis: its anatomical basis and itsclassification. Microsurgery. 1993;14:430–439.
Frostick SP, Yin Q, Kemp G. Schwann cells, neurotrophic factors and peripheral nerve regeneration. Microsurgery. 1998;18:397–405.
Blottner D, Baumgarten HG. Neurotrophy and regeneration in vivo. Acta Anat. 1994;150:235–245.
Sinis N, Kraus A, Tselis N, Haerle M, Werdin F, Schaller HE. Functional recovery after implantation of artificial nerve grafts in the rat—a systematic review. J Brachial Plex Peripher Nerve Inj. 2009 Oct 25;4:19. doi:10.1186/1749-7221-4-19. PubMed PMID: 19852862; PubMed Central PMCID: PMC2770034.
Liu H, Yao F, Zhou Y et al. Porous poly (DL-lactic acid) modified chitosan-gelatin scaffolds for tissue engineering. J Biomater. Appl. 2005;19(4):303–322.
Pabari A, Yang SY, Mosahebi A, Seifalian AM. Recent advances in artificial nerve conduit design: strategies for the delivery of luminal fillers. J Control Release. 2011 Nov 30;156(1):2–10. doi:10.1016/j.jconrel.2011.07.001. Epub 2011 Jul 6. Review. PubMed PMID: 21763371.
Labrador RO, Buti M, Navarro IX. Influence of collagen and laminin gels concentration on nerve regeneration after resection and tube repair. Exp Neurol. 1998:149(1):243–252.
Mosahebi A, Wiberg M, Terenghi G. Addition of fibronectin to alginate matrix improves peripheral nerve regeneration in tissue-engineered conduits. Tissue Eng. 2003;9(2):209–218.
Adams DN, Kao EY, Hypolite CL, Distefano MD, Hu WS, Letourneau PC. Growth cones turn and migrate up an immobilized gradient of the laminin IKVAV peptide. J Neurobiol 2005;62:134–147 [PubMed: 15452851].
Dodla MC, Bellamkonda RV. Anisotropic scaffolds facilitate enhanced neurite extension in vitro. J Biomed Mater Res A. 2006;78A:213–221 [PubMed: 16892507].
Mazal PR, Millesi H. Neurolysis: is it beneficial or harmful? Acta Neurochir. 2005;92(Suppl):3–6.
Ho WS, Ying SY, Chan PC, Chan HH. Use of onion extract, heparin, allantoin gel in prevention of scarring in chinese patients having laser removal of tattoos: a prospective randomized controlled trial. Dermatol Surg. 2006 Jul;32(7):891–6. PubMed PMID: 16875470.
Kahraman A, Kahveci R. Evaluating the effect of polytetrafluoroethylene and extractum cepae-heparin-allantoin gel in peripheral nerve injuries in a rat model. Plast Surg (Oakv). 2015 Spring;23(1):9–14. PubMed PMID: 25821766; PubMed Central PMCID: PMC4364148.
Billings PC, Pacifici M. Interactions of signaling proteins, growth factors and other proteins with heparan sulfate: mechanisms and mysteries. Connect Tissue Res. 2015;56(4):272–80. doi:10.3109/03008207.2015.1045066.
Olczyk P, Mencner Ł, Komosinska-Vassev K. Diverse roles of heparan sulfate and heparin in wound repair. Biomed Res Int. 2015;2015:549417. doi:10.1155/2015/549417. Epub 2015 Jul 7. Review. PubMed PMID: 26236728; PubMed Central PMCID: PMC4508384.
Santos-Silva A, Fairless R, Frame MC, Montague P, Smith GM, Toft A, Riddell JS, Barnett SC. FGF/heparin differentially regulates Schwann cell and olfactory ensheathing cell interactions with astrocytes: a role in astrocytosis. J Neurosci. 2007 Jul 4;27(27):7154–7167.
Yiu G, He Z. Glial inhibition of CNS axon regeneration. Nat Rev Neurosci. 2006;7:617–627.
Bradbury EJ, Moon LD, Popat RJ, King VR, Bennett GS, Patel PN, Fawcett JW, McMahon SB. Chondroitinase ABC promotes functional recovery after spinal cord injury. Nature. 2002;416:636–640 [PubMed: 11948352].
Houle JD, Tom VJ, Mayes D, Wagoner G, Phillips N, Silver J. Combining an autologous peripheral nervous system “bridge” and matrix modification by chondroitinase allows robust, functional regeneration beyond a hemisection lesion of the adult rat spinal cord. J Neurosci. 2006 Jul 12;26(28):7405–7415.
Jain A, Kim YT, McKeon RJ, Bellamkonda RV. In situ gelling hydrogels for conformal repair of spinal cord defects and local delivery of BDNF after spinal cord injury. Biomaterials. 2006;27:497–504 [PubMed: 16099038].
Carraro U, Boncompagni S, Gobbo V, Rossini K, Zampieri S, Mosole S, Ravara B, Nori A, Stramare R, Ambrosio F, Piccione F, Masiero S, Vindigni V, Gargiulo P, Protasi F, Kern H, Pond A, Marcante A. Persistent muscle fiber regeneration in long term denervation. Past, present, future. Eur J Transl Myol. 2015 Mar 11;25(2):4832. doi:10.4081/ejtm.2015.4832. eCollection 2015 Mar 11. Review. PubMed PMID: 26913148; PubMed Central PMCID: PMC4383182.
Brenner HR, Lomo T, Williamson R. Control of end-plate channel properties by neurotrophic effects andby muscle activity in rat. J Physiol. 1987;388:367–381.
Han H, Ao Q, Chen G, Wang S, Zuo H. A novel basic fibroblast growth factor delivery system fabricated with heparin-incorporated fibrin-fibronectin matrices for repairing rat sciatic nerve disruptions. Biotechnol Lett. 2010 Apr;32(4):585–91. doi:10.1007/s10529-009-0186-z. Epub 2009 Dec 24. PubMed PMID: 20033834.
McKay Hart A, Wiberg M, Terenghi G. Exogenous leukaemia inhibitory factor enhances nerve regeneration after late secondary repair using a bioartif icial nerve conduit. Br J Plast Surg. 2003;56(5):444–450.
Neufeld G, Gospodarowicz D, Dodge L, Fujii DK. Heparin modulation of the neurotropic effects of acidic and basic f ibroblast growth factors and nerve growth factor on PC12 cells. J Cell Physiol. 1987;131(1):131–140.
Rider CC. Interaction between glial-cell-line-derived neurotrophic factor (GDNF) and 2-O-sulphated heparin-related glycosaminoglycans. Biochem Soc Trans. 2003;31(2):337–339.
Barnett MW, FisherCE, Perona-Wright G, Davies JA. Signalling by glial cell linederived neurotrophic factor (GDNF) requires heparan sulphate glycosaminoglycan. J Cell Sci. 2002;115(Pt 23):4495–4503.
Tanaka M, Xiao H, Kiuchi K. Heparin facilitates glial cell line-derived neurotrophic factor signal transduction. Neuroreport. 2002;13(15):1913–1916.
Sakiyama-Elbert SE, Hubbell JA. Controlled release of nerve growth factor from a heparin-containing fibrin-based cell ingrowth matrix. J Control Release. 2000;69(1):149–158.
Wood MD, Hunter D, Mackinnon SE, Sakiyama–Elbert SE. Heparin–binding-affinity-based delivery systems releasing nerve growth factor enhance sciatic nerve regeneration. J Biomater Sci Polym Ed. 2010;21(6):771–787.
Amr S, Amr H. Bridging defects in chronic spinal cord injury using peripheral nerve grafts; results of indwelling catheter implantation; a comparative clinical study. In: Research on complication—current issues and technology. ISBN 978-1-922227-37-9. iConcept Press Limited, Brisbane, Australia; 2016.
Amr S. Bridging defects in chronic spinal cord injury using peripheral nerve grafts: nerve grafting techniques and overcoming the gliosis; from basic science to clinical experience. In: Fuller H (editor) Recovery of motor function following spinal cord injury. Intechopen, Croatia, EU. 2016.
Georgiou M, Bunting SCJ, Davies HD, Loughlin AJ, Golding JP, Phillips JB. Engineered neural tissue for peripheral nerve repair. Biomaterials. 2013;34:7335–7343.
Benoit JP, Faisant N, Venier-Julienne MC, Menei P. Development of micro-spheres for neurological disorders: from basics to clinical applications. J Control Release. 2000;65:285–296 [PubMed:10699288].
Haastert-Talini K, Geuna S, Dahlin LB, Meyer C, Stenberg L, Freier T, Heimann C, Barwig C, Pinto LF, Raimondo S, Gambarotta G, Samy SR, Sousa N, Salgado AJ, Ratzka A, Wrobel S, Grothe C. Chitosan tubes of varying degrees of acetylation for bridging peripheral nerve defects. Biomaterials. 2013 Dec;34(38):9886–904. doi:10.1016/j.biomaterials.2013.08.074. Epub 2013 Sep 17. PubMed PMID: 24050875.
Yuan Y, Zhang P, Yang Y, Wang X, Gu X. The interaction of Schwann cells with chitosan membranes and fibers in vitro. Biomaterials. 2004;25(18):4273–4278 [PubMed: 15046917].
Yang Y, Liu M, Gu Y, Lin S, Ding F, Gu X. Effect of chitooligosaccharide on neuronal differentiation of PC-12 cells. Cell Biol Int. 2009;33(3):352–356.
Wang Y, Zhao Y, Sun C, Hu W, Zhao J, Li G, Zhang L, Liu M, Liu Y, Ding F, Yang Y, Gu X. Chitosan degradation products promote nerve regeneration by stimulating Schwann cell proliferation via miR-27a/FOXO1 axis. Mol Neurobiol. 2014 Nov 18 [Epub ahead of print] doi:10.1007/s12035-014-8968-2.
Kusaba H, Terada-Nakaishi M, Wang W, Itoh S, Nozaki K, Nagai A, Ichinose S, Takakuda K. Comparison of nerve regenerative efficacy between decellularized nerve graft and nonwoven chitosan conduit. Biomed Mater Eng. 2016 May12;27(1):75–85. doi:10.3233/BME-161571. PubMed PMID: 27175469.
Wrobel S, Serra SC, Ribeiro-Samy S, Sousa N, Heimann C, Barwig C, Grothe C, Salgado AJ, Haastert-Talini K. In vitro evaluation of cell-seeded chitosan films for peripheral nerve tissue engineering. Tissue Eng Part A. 2014 Sep;20(17–18):2339–2349.
Stenberg L, Kodama A, Lindwall-Blom C, Dahlin LB. Nerve regeneration in chitosan conduits and in autologous nerve grafts in healthy and in type 2 diabetic Goto-Kakizaki rats. Eur J Neurosci. 2016 Feb;43(3):463–73. doi:10.1111/ejn.13068. Epub 2015 Nov 2. PubMed PMID: 26355640.
Gonzalez-Perez F, Cobianchi S, Geuna S, Barwig C, Freier T, Udina E, Navarro X. Tubulization with chitosan guides for the repair of long gap peripheral nerve injury in the rat. Microsurgery. 2015 May;35(4):300–308. doi:10.1002/micr.22362.Epub 2014 Dec 4. PubMed PMID: 25471200.
Meyer C, Stenberg L, Gonzalez-Perez F, Wrobel S, Ronchi G, Udina E, Suganuma S, Geuna S, Navarro X, Dahlin LB, Grothe C, Haastert-Talini K. Chitosan-film enhanced chitosan nerve guides for long-distance regeneration of peripheral nerves. Biomaterials. 2016 Jan;76:33–51. doi:10.1016/j.biomaterials.2015.10.040. Epub 2015 Oct 21. PubMed PMID: 26517563.
Hsu SH, Lu PS, Ni HC, Su CH. Fabrication and evaluation of microgrooved polymers as peripheral nerve conduits. Biomed Microdevices. 2007 Oct;9(5):665–74. PubMed PMID: 17562182.
Zhang YG, Huang JH, Hu XY, Sheng QS, Zhao W, Luo ZJ. Omentum-wrapped scaffold with longitudinally oriented micro-channels promotes axonal regeneration and motor functional recovery in rats. PLoS One. 2011;6(12):e29184. doi:10.1371/journal.pone.0029184.
Hu X, Huang J, Ye Z, Xia L, Li M, Lv B, Shen X, Luo Z. A novel scaffold with longitudinally oriented microchannels promotes peripheral nerve regeneration. Tissue Eng Part A. 2009 Nov;15(11):3297–308. doi:10.1089/ten.TEA.2009.0017. PubMed PMID: 19382873.
Hu W, Gu J, Deng A, Gu X. Polyglycolic acid filaments guide Schwann cell migration in vitro and in vivo. Biotechnol Lett. 2008 Nov;30(11):1937–42. doi:10.1007/s10529–008–9795–1. Epub 2008 Jul 9. PubMed PMID: 18612593.
Patel M, Mao L, Wu B, Vandevord PJ. GDNF-chitosan blended nerve guides: a functional study. J Tissue Eng Regen Med. 2007 Sep-Oct;1(5):360–7. PubMed PMID:18038430.
Huang YC, Huang CC, Huang YY, Chen KS. Surface modification and characterization of chitosan or PLGA membrane with laminin by chemical and oxygen plasma treatment for neural regeneration. J Biomed Mater Res A. 2007 Sep15;82(4):842–51. PubMed PMID: 17335016.
Prabhakaran MP, Venugopal JR, Chyan TT, Hai LB, Chan CK, Lim AY, Ramakrishna S. Electrospun biocomposite nanofibrous scaffolds for neural tissue engineering. Tissue Eng Part A. 2008 Nov;14(11):1787–97. doi:10.1089/ten.tea.2007.0393. PubMed PMID: 18657027.
Huang C, Chen R, Ke Q, Morsi Y, Zhang K, Mo X. Electrospun collagen-chitosan-TPU nanofibrous scaffolds for tissue engineered tubular grafts. Colloids Surf B Biointerfaces. 2011 Feb 1;82(2):307–15. doi:10.1016/j.colsurfb.2010.09.002.
Wang W, Itoh S, Matsuda A, Ichinose S, Shinomiya K, Hata Y, Tanaka J. Influences of mechanical properties and permeability on chitosan nano/microfiber mesh tubes as a scaffold for nerve regeneration. J Biomed Mater Res A. 2008 Feb;84(2):557–66 (Erratum in: J Biomed Mater Res A. 2008 Mar 1;84(3):846) PubMed PMID: 17941013.
Junka R, Valmikinathan CM, Kalyon DM, Yu X. Laminin functionalized biomimetic nanofibers for nerve tissue engineering. J Biomater Tissue Eng. 2013 Aug 1;3(4):494–502. PubMed PMID: 24083073; PubMed Central PMCID: PMC3785102.
Duda S, Dreyer L, Behrens P, Wienecke S, Chakradeo T, Glasmacher B, Haastert-Talini K. Outer electrospun polycaprolactone shell induces massive foreign body reaction and impairs axonal regeneration through 3D multichannel chitosan nerve guides. Biomed Res Int. 2014;2014:835269. doi:10.1155/2014/835269. Epub 2014 Apr 9. PubMed PMID: 24818158; PubMed Central PMCID: PMC4000981.
H P S AK, Saurabh CK, A S A, Nurul Fazita MR, Syakir MI, Davoudpour Y, Rafatullah M, Abdullah CK, M Haafiz MK, Dungani R. A review on chitosan-cellulose blends and nanocellulose reinforced chitosan biocomposites: properties and their applications. Carbohydr Polym. 2016 Oct 5;150:216–26. doi:10.1016/j.carbpol.2016.05.028. Epub 2016 May 14. Review.
Itoh S, Suzuki M, Yamaguchi I, Takakuda K, Kobayashi H, Shinomiya K, Tanaka J. Development of a nerve scaffold using a tendon chitosan tube. Artif Organs. 2003 Dec;27(12):1079–88. PubMed PMID: 14678421.
Itoh S, Yamaguchi I, Suzuki M, Ichinose S, Takakuda K, Kobayashi H, Shinomiya K, Tanaka J. Hydroxyapatite-coated tendon chitosan tubes with adsorbed laminin peptides facilitate nerve regeneration in vivo. Brain Res. 2003 Dec 12;993(1–2):111–23. PubMed PMID: 14642836.
Xue C, Hu N, Gu Y, Yang Y, Liu Y, Liu J, Ding F, Gu X. Joint use of a chitosan/PLGA scaffold and MSCs to bridge an extra large gap in dog sciatic nerve. Neurorehabil Neural Repair. 2012 Jan;26(1):96–106. doi:10.1177/1545968311420444.
Nomura H, Zahir T, Kim H, Katayama Y, Kulbatski I, Morshead CM, Shoichet MS, Tator CH. Extramedullary chitosan channels promote survival of transplanted neural stem and progenitor cells and create a tissue bridge after complete spinal cord transection. Tissue Eng A 2008b;14:649–665.
Yue W, Yan F, Zhang YL, Liu SL, Hou SP, Mao GC, Liu N, Ji Y. Differentiation of rat bone marrow mesenchymal stem cells into neuron-like cells in vitro and co-cultured with biological scaffold as transplantation carrier. Med Sci Monit. 2016 May 26;22:1766–1772. PubMed PMID: 27225035.
Zhu L, Liu T, Cai J, Ma J, Chen AM. Repair and regeneration of lumbosacral nerve defects in rats with chitosan conduits containing bone marrow mesenchymal stem cells. Injury. 2015 Nov;46(11):2156–63. doi:10.1016/j.injury.2015.08.035. Epub 2015 Sep 1. PubMed PMID: 26429103.
Hu N, Wu H, Xue C, Gong Y, Wu J, Xiao Z, Yang Y, Ding F, Gu X. Long-term outcome of the repair of 50 mm long median nerve defects in rhesus monkeys with marrow mesenchymal stem cells-containing, chitosan-based tissue engineered nerve grafts. Biomaterials. 2013 Jan;34(1):100–11. doi:10.1016/j.biomaterials.2012.09.020. Epub 2012 Oct 11. PubMed PMID: 23063298.
Itoh S, Matsuda A, Kobayashi H, Ichinose S, Shinomiya K and Tanaka J. Effects of a laminin peptide (YIGSR) immobilized on crab-tendon chitosan tubes on nerve regeneration. J Biomed Mater Res Part B Appl Biomater. 2005;73(2):375–382.
Hsu SH, Kuo WC, Chen YT, Yen CT, Chen YF, Chen KS, Huang WC, Cheng H. New nerve regeneration strategy combining laminin-coated chitosan conduits and stem cell therapy. Acta Biomater. 2013 May;9(5):6606–15. doi:10.1016/j.actbio.2013.01.025. Epub 2013 Feb 1. PubMed PMID: 23376237.
Wang X, Li Y, Gao Y, Chen X, Yao J, Lin W, Chen Y, Liu J, Yang Y, Wang X. Combined use of spinal cord-mimicking partition type scaffold architecture and neurotrophin-3 for surgical repair of completely transected spinal cord in rats. J Biomater Sci Polym Ed. 2013;24(8):927–39. doi:10.1080/09205063.2012.727267. Epub 2012 Oct 2. PubMed PMID: 23647249.
Nie X, Deng M, Yang M, Liu L, Zhang Y, Wen X. Axonal regeneration and remyelination evaluation of chitosan/gelatin-based nerve guide combined with transforming growth factor-β1 and Schwann cells. Cell Biochem Biophys. 2014 Jan;68(1):163–72.
Yang Y, Gu X, Tan R, Hu W, Wang X, Zhang P, Zhang T. Fabrication and properties of a porous chitin/chitosan conduit for nerve regeneration. Biotechnol Lett 2004; 26(23): 1793–1797
Yang YM, Hu W, Wang XD, Gu XS. The controlling biodegradation of chitosan fibers by N-acetylation in vitro and in vivo. J Mater Sci Mater Med. 2007;18(11):2117–2121.
Yang Y, Zhao W, He J, Zhao Y, Ding F, Gu X. Nerve conduits based on immobilization of nerve growth factor onto modified chitosan by using genipin as a crosslinking agent. Eur J Pharm Biopharm. 2011;79(3):519–525.
Yan F, Yue W, Zhang YL, Mao GC, Gao K, Zuo ZX, Zhang YJ, Lu H. Chitosan-collagen porous scaffold and bone marrow mesenchymal stem cell transplantation for ischemic stroke. Neural Regen Res. 2015 Sep;10(9):1421–1426.
Meyer C, Wrobel S, Raimondo S, Rochkind S, Heimann C, Shahar A, Ziv-Polat O, Geuna S, Grothe C, Haastert-Talini K. Peripheral nerve regeneration through hydrogel-enriched chitosan conduits containing engineered schwann cells for drug delivery. Cell Transplant. 2016;25(1):159–182. doi:10.3727/096368915X688010. Epub2015 Apr 14. PubMed PMID: 25876520.
Jiang M, Cheng Q, Su W, Wang C, Yang Y, Cao Z, Ding F. The beneficial effect of chitooligosaccharides on cell behavior and function of primary Schwann cells is accompanied by up-regulation of adhesion proteins and neurotrophins. Neurochem Res. 2014 Nov;39(11):2047–2057.
Hoveizi E, Tavakol S, Ebrahimi-Barough S. Neuroprotective effect of transplanted neural precursors embedded on PLA/CS scaffold in an animal model of multiple sclerosis. Mol Neurobiol. 2015;51(3):1334–1342.
Zhang P, Xu H, Zhang D, Fu Z, Zhang H, Jiang B. The biocompatibility research of functional Schwann cells induced from bone mesenchymal cells with chitosan conduit membrane. Artif Cells Blood Substit Immobil Biotechnol. 2006;34(1):89–97. PubMed PMID: 16519406.
Skop NB, Calderon F, Levison SW, Gandhi CD, Cho CH. Heparin crosslinked chitosan microspheres for the delivery of neural stem cells and growth factors for central nervous system repair. Acta Biomater. 2013 Jun;9(6):6834–43. doi:10.1016/j.actbio.2013.02.043. Epub 2013 Mar 5. PubMed PMID: 23467042.
Wei Y, Gong K, Zheng Z, Wang A, Ao Q, Gong Y, Zhang X. Chitosan/silk fibroin-based tissue-engineered graft seeded with adipose-derived stem cells enhances nerve regeneration in a rat model. J Mater Sci Mater Med. 2011 Aug;22(8):1947–64. doi:10.1007/s10856-011-4370-z. Epub 2011 Jun 8. PubMed PMID: 21656031.
Wang W, Itoh S, Konno K, Kikkawa T, Ichinose S, Sakai K, Ohkuma T, Watabe K. Effects of Schwann cell alignment along the oriented electrospun chitosan nanofibers on nerve regeneration. J Biomed Mater Res A. 2009 Dec 15;91(4):994–1005. doi:10.1002/jbm.a.32329. PubMed PMID: 19097155.
Maysinger D, Krieglstein K, Filipovic-Grcic J, Sendtner M, Unsicker K, Richardson P. Microencapsulated ciliary neurotrophic factor: physical properties and biological activities. Exp Neurol. 1996 Apr;138(2):177–88. PubMed PMID: 8620916.
Raisi A, Azizi S, Delirezh N, Heshmatian B, Farshid AA, Amini K. The mesenchymal stem cell-derived microvesicles enhance sciatic nerve regeneration in rat: a novel approach in peripheral nerve cell therapy. J Trauma Acute Care Surg. 2014 Apr;76(4):991–7. doi:10.1097/TA.0000000000000186. PubMed PMID: 24662862.
Qi F, Wang Y, Ma T, Zhu S, Zeng W, Hu X, Liu Z, Huang J, Luo Z. Electricalregulation of olfactory ensheathing cells using conductive polypyrrole/chitosanpolymers. Biomaterials. 2013 Feb;34(7):1799–809. doi:10.1016/j.biomaterials.2012.11.042. Epub 2012 Dec 7. PubMed PMID: 23228424.
Liu Z, Huang L, Liu L, Luo B, Liang M, Sun Z, Zhu S, Quan X, Yang Y, Ma T, Huang J, Luo Z. Activation of Schwann cells in vitro by magnetic nanocomposites via applied magnetic field. Int J Nanomedicine. 2014 Dec 17;10:43–61. doi:10.2147/IJN.S74332. eCollection 2015. PubMed PMID: 25565803; PubMed CentralPMCID: PMC4275057.
Gasperini L, Mano JF, Reis RL. Natural polymers for the microencapsulation of cells. J R Soc Interface. 2014;11:0817. doi:10.1098/rsif.2014.0817
Stokols S, Tuszynski MH. The fabrication and characterization of linearly oriented nerve guidance scaffolds for spinal cord injury. Biomaterials. 2004;25:5839–5846.
Stokols S, Sakamoto J, Breckon C, Holt T, Weiss J, Tuszynski MH, Templated agarose scaffolds support linear axonal regeneration. Tissue Eng. 2006;12:2777–2787.
Stokols S, Tuszynski MH. Freeze-dried agarose scaffolds with uniaxial channels stimulate and guide linear axonal growth following spinal cord injury. Biomaterials. 2006;27:443–451.
Tabesh H, Amoabediny G, Nik NS, Heydari M, Yosefifard M, Siadat SO, Mottaghy K. The role of biodegradable engineered scaffolds seeded with Schwann cells for spinal cord regeneration. Neurochem Int. 2009;54:73–83 [PubMed: 19084565].
Sachlos E, Czernuszka JT. Making tissue engineering scaffolds work. Review: the application of solid freeform fabrication technology to the production of tissue engineering scaffolds. Eur Cell Mater. 2003;5:29–39 [PubMed: 14562270].
Koffler J, Samara RF, Rosenzweig ES. Using templated agarose scaffolds to promote axon regeneration through sites of spinal cord injury. Methods Mol Biol. 2014;1162:157–165. doi:10.1007/978-1-4939-0777-9_13. PubMed PMID: 24838966.
Khaing ZZ, Schmidt CE. Advances in natural biomaterials for nerve tissue repair. Neurosci Lett. 2012 Jun 25;519(2):103–114.
Dodla MC, Bellamkonda RV. Differences between the effect of anisotropic and isotropic laminin and nerve growth factor presenting scaffolds on nerve regeneration across long peripheral nerve gaps. Biomaterials. 2008 Jan;29(1):33–46.
Cullen DK, Tang-Schomer MD, Struzyna LA, Patel AR, Johnson VE, Wolf JA, Smith DH. Microtissue engineered constructs with living axons for targeted nervous system reconstruction. Tissue Eng Part A. 2012 Nov;18(21–22):2280–9. doi:10.1089/ten.TEA.2011.0534
Gros T, Sakamoto JS, Blesch A, Havton LA, Tuszynski MH. Regeneration of long-tract axons through sites of spinal cord injury using templated agarose scaffolds. Biomaterials. 2010 Sep;31(26):6719–6729. doi:10.1016/j.biomaterials.2010.04.035
Chvatal SA, Kim YT, Bratt-Leal AM, Lee H, Bellamkonda RV. Spatial distribution and acute anti–inflammatory effects of Methylprednisolone after sustained local delivery to the contused spinal cord. Biomaterials 2008;29:1967–1975 [PubMed: 18255138].
Wylie RG, Ahsan S, Aizawa Y, Maxwell KL, Morshead CM, Shoichet MS. Spatially controlled simultaneous patterning of multiple growth factors in three-dimensional hydrogels. Nat Mater. 2011;10:799–806.
Cardoso MJ, Costa RR, Mano JF. Marine origin polysaccharides in drug delivery systems. Mar Drugs. 2016 Feb 5;14(2). pii: E34. doi:10.3390/md14020034. Review. PubMed PMID: 26861358; PubMed Central PMCID: PMC4771987.
Lu HF, Lim SX, Leong MF, Narayanan K, Toh RP, Gao S, Wan AC. Efficient neuronal differentiation and maturation of human pluripotent stem cells encapsulated in 3D microfibrous scaffolds. Biomaterials. 2012 Dec;33(36):9179–9187.
Suzuki K, Suzuki Y, Tanihara M, Ohnishi K, Hashimoto T, Endo K, Nishimura Y. Reconstruction of rat peripheral nerve gap without sutures using freezedried alginate gel. J Biomed Mater Res. 2000;49:528–533.
Sufan W, Suzuki Y, Tanihara M, Ohnishi K, Suzuki K, Endo K, Nishimura Y. Sciatic nerve regeneration through alginate with tubulation or nontubulation repair in cat. J Neurotrauma. 2001;18:329–338.
Park JH, Min J, Baek SR, Kim SW, Kwon IK, Jeon SR. Enhanced neuroregenerative effects by scaffold for the treatment of a rat spinal cord injury with Wnt3a-secreting fibroblasts. Acta Neurochir (Wien). 2013 May;155(5):809–16. doi:10.1007/s00701-013-1663-7
Pfister LA, Alther E, Papaloizos M, Merkle HP, Gander B. Controlled nerve growth factor release from multi-ply alginate/chitosan-based nerve conduits. Eur J Pharm Biopharm. 2008;69(2):563–572.
Suzuki Y, Ishikawa N, Tanihara M, Saito S. Nontubulation repair of peripheral nerve gap using heparin/alginate gel combined with b-FGF. Plast Reconstr Surg Glob Open. 2016 Feb 5;4(1):e600. doi:10.1097/GOX.0000000000000581. eCollection 2016 Jan. PubMed PMID: 27104099; PubMed Central PMCID: PMC4801089.
Tanihara M, Suzuki Y, Yamamoto E, Noguchi A, Mizushima Y. Sustained release of basic fibroblast growth factor and angiogenesis in a novel covalently crosslinked gel of heparin and alginate. J Biomed Mater Res. 2001 Aug;56(2):216–21. PubMed PMID: 11340591.
Szarek D, Marycz K, Bednarz P, Tabakow P, Jarmundowicz W, Laska J. Influence of calcium alginate on peripheral nerve regeneration: in vivo study. Biotechnol Appl Biochem. 2013 Nov-Dec;60(6):547–556. doi:10.1002/bab.1096. Epub 2013 Aug 3. PubMed PMID: 23909973.
Ohta M, Suzuki Y, Chou H, Ishikawa N, Suzuki S, Tanihara M, Suzuki Y, Mizushima Y, Dezawa M, Ide C. Novel heparin/alginate gel combined with basic fibroblast growth factor promotes nerve regeneration in rat sciatic nerve. J Biomed Mater Res A. 2004;71(4):661–668.
Mohanna PN, Terenghi G, Wiberg M. Composite PHB-GGF conduit for long nerve gap repair: a long-term evaluation. Scand J Plast Reconstr Surg Hand Surg. 2005;39(3):129–137. PubMed PMID: 16019744.
Mohanna PN, Young RC, Wiberg M, Terenghi G. A composite poly-hydroxybutyrate-glial growth factor conduit for long nerve gap repairs. J Anat. 2003 Dec;203(6):553–565.
Mosahebi A, Simon M, Wiberg M, Terenghi G. A novel use of alginate hydrogel as Schwann cell matrix. Tissue Eng. 2001;7(5):525–534.
Mosahebi A, Fuller P, Wiberg M, Terenghi G. Effect of allogeneic Schwann celltransplantation on peripheral nerve regeneration. Exp Neurol. 2002 Feb;173(2):213–223. PubMed PMID: 11822885.
Quigley AF, Bulluss KJ, Kyratzis IL, Gilmore K, Mysore T, Schirmer KS, Kennedy EL, O’Shea M, Truong YB, Edwards SL, Peeters G, Herwig P, Razal JM, Campbell TE, Lowes KN, Higgins MJ, Moulton SE, Murphy MA, Cook MJ, Clark GM, Wallace GG, Kapsa RM. Engineering a multimodal nerve conduit for repair of injured peripheral nerve. J Neural Eng. 2013 Feb;10(1):016008.
Zhao H, Yang BL, Liu ZX, Yu Q, Zhang WJ, Yuan K, Zeng HH, Zhu GC, Liu DM, Li Q. Microencapsulation improves inhibitory effects of transplanted olfactory ensheathing cells on pain after sciatic nerve injury. Neural Regen Res. 2015Aug;10(8):1332–1337.
Francis NL, Shanbhag MS, Fischer I, Wheatley MA. Influence of alginate cross-linking method on neurite response to microencapsulated neurotrophin-producing fibroblasts. J Microencapsul. 2011;28(5):353–362.
Song M, Chen SZ, Han H, Xiong Y. An experimental study on repair of peripheral nerve injury by transplantation of microcapsulated NGF-expressing NIH 3T3 cells. Zhonghua Zheng Xing Wai Ke Za Zhi. 2005 Jan;21(1):53–7. Chinese.PubMed PMID: 15844601.
Sanna V, Roggio AM, Siliani S, et al. Development of novel cationic chitosan-and anionic alginate–coated poly(d, l-lactide-co-glycolide) nanoparticles for controlled release and light protection of resveratrol. Int J Nanomed. 2012;7:5501–5516.
Takka S, Gürel A. Evaluation of chitosan/alginate beads using experimental design: formulation and in vitro characterization. AAPS PharmSciTech. 2010;11(1):460–466. doi:10.1208/s12249–010–9406-z.